Structural, Electronic, and Magnetic Properties of UFeS3 and UFeSe3
Geng Bang Jin; Emilie Ringe; Gary J. Long; Fernande Grandjean; Moulay T. Sougrati; Eun Sang Choi; Daniel M. Wells; Mahalingam Balasubramanian; James A. Ibers; Inorganic Chemistry 49 (2010) 10455–10467; doi:10.1021/ic101474e

data_4317030
_publ_section_title
;
 Structural, Electronic, and Magnetic Properties of UFeS3 and UFeSe3
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              10455
_journal_page_last               10467
_journal_paper_doi               10.1021/ic101474e
_journal_volume                  49
_journal_year                    2010
_chemical_formula_moiety         'U Fe S3'
_chemical_formula_sum            'Fe S3 U'
_chemical_formula_weight         390.06
_chemical_name_common            'Uranium iron sulfide'
_chemical_name_systematic
; 

 ? 

;
_space_group_IT_number           63
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   3.80090(10)
_cell_length_b                   11.6148(4)
_cell_length_c                   8.7022(3)
_cell_measurement_reflns_used    1979
_cell_measurement_temperature    296(2)
_cell_measurement_theta_max      28.42
_cell_measurement_theta_min      2.92
_cell_volume                     384.17(2)
_computing_cell_refinement       'APEX2 v2.0-2 (Bruker, 2005)'
_computing_data_collection       'APEX2 v2.1-4 (Bruker, 2007)'
_computing_data_reduction        'SAINT version 7.23a (Bruker, 2005)'
_computing_molecular_graphics    'CrystalMaker for Windows ver. 2.0.6 (2008)'
_computing_publication_material  'SHELXTL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      296(2)
_diffrn_measured_fraction_theta_full 0.966
_diffrn_measured_fraction_theta_max 0.966
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0192
_diffrn_reflns_av_sigmaI/netI    0.0102
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       -5
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            2198
_diffrn_reflns_theta_full        28.45
_diffrn_reflns_theta_max         28.45
_diffrn_reflns_theta_min         3.51
_exptl_absorpt_coefficient_mu    47.256
_exptl_absorpt_correction_T_max  0.2805
_exptl_absorpt_correction_T_min  0.0385
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   'faces indexed'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    6.744
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             664
_exptl_crystal_size_max          0.354
_exptl_crystal_size_mid          0.040
_exptl_crystal_size_min          0.031
_refine_diff_density_max         1.511
_refine_diff_density_min         -1.539
_refine_diff_density_rms         0.357
_refine_ls_extinction_coef       0.0074(5)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.417
_refine_ls_matrix_type           full
_refine_ls_number_parameters     20
_refine_ls_number_reflns         285
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.417
_refine_ls_R_factor_all          0.0149
_refine_ls_R_factor_gt           0.0149
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
; calc 

 [1.00000+0.00000exp(0.00(sin\q/\l)^2^)]/ 

   [\s^2^(Fo^2^)+0.0000+0.0000*P+(0.0269P)^2^+0.0000sin\q/\l] 

 where P = 1.00000Fo^2^ + 0.00000Fc^2^ 

;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0430
_refine_ls_wR_factor_ref         0.0430
_reflns_number_gt                285
_reflns_number_total             285
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic101474e_si_002_4.cif
_cod_data_source_block           UFeS3296K
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_database_code               4317030